UNIVERSITY OF NAPLES FEDERICO II
Department of Chemical, Materials and Industrial Production Engineering
Ph.D COURSE IN MATERIALS ENGINEERING AND STRUCTURES XXV CYCLE
“ENGINEERING PATTERNED SURFACES TO CONTROL CELL BEHAVIOUR”
Prof. Paolo Antonio Netti Carlo Fortunato Natale Prof. Maurizio Ventre
Prof. Giuseppe Mensitieri
March 2010 - March 2013
TABLE OF CONTENTS
Chapter 1 ... 5
Introduction ... 5
1.1 Tissue engineering ... 5
1.2 Cell Instructive Materials ... 7
1.3 The Focal Adhesion ... 8
1.4 Cell Cytoskeleton ... 10
1.5 Mechanosensing ... 12
1.6 Substrate Topography ... 13
1.7 Aims and outcomes ... 14
1.8 References ... 16
Chapter 2 ... 21
Molding Micropatterns of Elasticity on Peg-Based Hydrogels to Control Cell Adhesion and Migration ... 21
2.1 Experimental ... 23
Hydrogel Preparation and Characterization ... 23
Micrometer Hydrogel Stamp Fabrication ... 24
2D Microelasticity Pattern Fabrication by the FIMIC Process ... 25
Atomic Force Microscopy (AFM) ... 26
Fibroblast Cell Culture ... 26
Immunological Staining ... 27
Optical and Fluorescent Microscopy ... 27
Field Emission Scanning Electron Microscopy (FESEM) ... 27
Cell Migration Experiments ... 27
2.3 Results and Discussion ... 28
2.4 Conclusions ... 35
2.5 References ... 37
Chapter 3 ... 39
Influence of nanotopography on focal adhesions, cytoskeleton assembly and nuclear shape ... 39
3.1 Experimental ... 41
Preparation of nanopatterned substrates ... 41
Cell Culture ... 42
Immunofluorescence ... 42
Drug treatment ... 42
Live-cell confocal microscopy ... 43
Image analysis ... 43
3.2 Results ... 44
Topography alters cell shape and FA clustering ... 44
Nanopattern affects actin dynamics and cell polarization ... 48
Basal stress fibres do not affect nuclear polarization. ... 51
3.3 Discussion and conclusions ... 53
3.4 References ... 57
Chapter 4 ... 59
Microtopographies to control cell migration by interfering with surface probing and focal adhesion assembly ... 59
4.1 Experimental ... 61
Preparation of micropatterned substrates ... 61
Cell Culture ... 62
Spreading Area and Immunofluorescence analysis ... 62
Time Lapse experiments ... 63
4.2 Results ... 64
Early events in cell adhesion ... 64
Long times cell migration analysis ... 66
Adhesion and Cytoskeleton assemblies ... 68
4.3 Discussion ... 71
4.4 Conclusions ... 75
4.5 References ... 77
Chapter 5 ... 80
Build up order tissue ... 80
5.1 Experimental ... 81
Preparation of nanopatterned substrates ... 81
Cell Culture ... 81
Time Lapse experiments ... 82
5.2 Results ... 83
Nanogrooved subrate effects on cell migration ... 83
Nanograted PDMS substrate influences collagen deposition ... 84
Multilayered cell sheet as a guidance for cell migration ... 85
5.3 Discussion ... 87
5.4 Conclusion ... 89
5.5 References ... 90
Chapter 6 ... 92
Conclusions ... 92
6.1 References ... 94
Tissues injury can often result in a reduction or loss of tissue functions. This is mainly due to the formation of scar tissue at the site of injury with a modification of local mechanical and structural properties. A great number of pathological conditions require replacement therapies involving the use of medical implants [1-2]. During the past several years a large variety of materials have been used for the fabrication of these medical implants leading to the development of a new discipline named Tissue Engineering.
Tissue Engineering is defined as the interdisciplinary field applying the principles and methods of engineering and life sciences to fundamentally understand and develop biological substitutes to restore, maintain or improve tissue functions . This field combines the unique properties of cells and biomaterials to repair or regenerate damaged and injured tissues, obtaining the potential to provide a revolutionary method for helping to treat such injuries and the many currently incurable degenerative diseases [3-4-5]. More specifically, any tissue engineered end product attempts to mimic the function of natural tissue. Implant material induce a tissue response and a control of this physiological response plays a critical role for the long term function of a medical device when implanted in the body. So the natural circumstances of the specific tissue have to be fundamentally understood, in order to optimize the development of function biological substitute.
1.1 Tissue engineering
Tissue Engineering approaches are based on the paradigm that using three basic ‘tools’, cell, scaffold and soluble factors, it is possible to induce the re-generation of a new tissue. The purpose of tissue engineering research is very clear: establishing a new clinical technology that makes possible medical treatments for diseases that have been too difficult to be cured by existing methods.
Biological tissues basically consist of cells, signaling systems and extracellular matrix (ECM) .
The cells are the core of the tissue, however, in the absence of signaling systems and/or of the ECM can’t explicate their functions. ECM represents the substances produced by cells and excreted to the
synthesize new tissue but without a three dimensional guide, isolated cells are not able to reproduce a tissue with its whole complex architecture and therefore functions. Cell proliferation is not sufficient for the generation of large-sized tissues and organs which require a proper support to generate 3D complex structures. The support is called scaffold. The major function of scaffold is to assists proliferation, differentiation and biosynthesis. Third key factor of tissue engineering are soluble molecules like proteins and growth factors that promote and support cells in the regeneration of neotissues. A wide range of proteins play a key role in cells proliferation and differentiation. These proteins are endogenously secreted in the body by cells themselves (autocrine) or as a result of communication with surrounding cells (paracrine). The practical use of growth factors in tissue engineering or clinical settings is very delicate. Indeed many studies demonstrated the limits of the direct application of growth factor in site of regeneration owing to rapid denaturation of the growth factors or by rapid enzymatic digestion. The earliest clinical application of human cell in tissue engineering started around 1980 concerning skin tissue. Just some year later, a membrane was used to attempt the regeneration of periodontal and alveolar bone.
This membrane prevented fibroblast invasion and guided bone regeneration. In 1988 Vacanti et al.
studied cell transplantation using bioadsorbable synthetic polymer as scaffold.
Successful clinical trials of tissue engineering constructs have been reported in literature.
Nowadays, skin, cardiovascular, bone and cartilage are the major areas of tissue‐engineered replacements in clinical trials and applications [7-8-9-10]. Matsumura et al.  reported the application of tissue‐engineered systems in cardiovascular surgery on children with various complex heart diseases. In this work they described a treatment with autogenic cells were isolated, cultured and subsequently seeded on a biodegradable polymer scaffold of poly(glycolic acid) combined with poly(lactic acid‐ε‐caprolactone). The first operation was performed in May 1999, and over 40 patients were treated the following years. Post‐operative analysis revealed no complications related to the tissue engineering autograft.
Macchiarini et al. designed and implanted a tissue‐engineered airway . In this case, all donor cells and antigens of an allogenic donor trachea were removed to prevent an immune reaction of the host towards the donor material. Subsequently, they cultivated the matrix with autogenic cells and transplanted the cell‐seeded scaffold into the patients. Immediately, the tissue engineered trachea became functional and after 4 months, the scaffold still showed normal appearance and good mechanical properties.
However biomedical devices applications were not always successful both for inflammatory response activation and defective interaction between cell and devices itself.
Improvement of cell material interaction assumes a relevant role in integration of exogenous material in an attempt to minimize non functional tissue encapsulation [13-14].
1.2 Cell Instructive Materials
A decrease in cellular adhesion may be the origin of reduced biomedical devices biocompatibility. A mild adhesion induces both a destabilization of the implant and an inhibition of tissue regeneration . The mechanism of cell-material interactions is crucial for the successful outcome of tissue engineered implants. Therefore, they need to be thoroughly understood in order to achieve all the desired and regulated cellular responses.
A combination of biochemical and biophysical signals, including interfacial presentation of molecular, topographic and mechanical cues occurs when cell interact with material surfaces.
Adhesion, migration, proliferation and differentiation are the cell activities mostly influenced by material properties.
Specifically engineered surfaces displaying selected biofunctional groups or micrometer-scale patterns have been used in order to study signal interactions and control cell responses in a systematic way.
Advancements in chemistry, material science and nanotechnologies greatly improved the possibility to imprint many different signals, according to predefined spatial patterns. In particular, patterns of biochemical signals, topographies on different length scales and mechanical cues clearly revealed cells’ ability to ‘sense’ and ‘react’ to external stimuli.
The potential to pattern material properties with nanometric accuracy has lead to the development of the next generation of biomaterials with extended functionalities and bioactivity . Cell Instructive Materials (CIMs) are designed to control and to direct cell fate making use of complex commands or instructions of nanofeatures exhibited on the top of material surface. Realization of these attractive materials will lead to a deep understanding of the mechanisms that regulate cell- material interactions unravelling the unknown events that occurs on the boundary between cell membrane and material surface.
Adherent cells are complex, self-sustaining units  that require ECM anchorage in order to proliferate . Chemical and topographical substrate modifications constitute a tool to facilitate cellular adhesion  and tissue deposition. After implantation a cascade of biological events occurs following adhesive protein adsorption to a material surface.
First of all, cells probe extracellular environment, forming protrusion termed “lamellipodia” with which cells move and sense their surroundings. Lamellipodia are associated with thin actin-rich plasma- membrane protrusion, filopodia, that function as antennae for cell to probe extracellular environment . Once cell locates a site suitable for adhesion a signaling feedback pathway initiates integrin receptor clustering at the plasma membrane and adhesion plaque protein recruitment . Initial cell-substrate contact and filopodia exploration is followed by lamellipodia-mediated ruffling , membrane activity and cellular flattening and spreading 
all mediated by the development of cell-substrate contacts termed “Focal Adhesions” (FAs).
1.3 The Focal Adhesion
Cell interacts with substrate and communicates intracellularly via transmembrane proteins termed integrins. These adhesion receptors are recognized as the central regulators of cell–biomaterial interactions, which mediate adhesion to the extra cellular matrix .
Integrin receptors are composed of 2 subunit alfa-beta, non-covalently linked. 18α and 8β subunit have been found, which combine to form 24 distinct dimers that can interact specifically to peptide motifs (most notably the RGD tripeptide) in ECM adhesive proteins such as fibronectin, vitronectin and laminin . Integrin-RGD link transmits information in a bi-directional manner from the extracellular environment to the machinery of intracellular transcription.
Figure 1.1: The proteins of the focal adhesion plaque (Campbell, 2008)
After recognition of RGD domain integrin rapidly associate and clusterize at binding site connecting actin microfilaments the via adaptor proteins as talin, vinculin, paxillin, a-actinin and focal adhesion kinase (FAK) (fig 1.1).
Nascent adhesion may mature into larger molecular structure. This requires clustering of additional integrins dimmers which increases nascent adhesion dimension by recruitment of more cytoplasmatic adhesion protein. In particular the binding of vinculin to talin triggers the clustering of activated integrin and through vinculin tail this complex associates with actin filament.
Figure 1.2: Model of Focal Adhesion formation (Geiger B., 2009)
Figure 1.2 summarizes FA formation and maturation process. Focal complex originates as spot of 0,5 µm2 regulated by the GTPase Rac pathway . Formation of focal complex occurs underneath lamellipodium . Focal complex gradually matures into focal adhesion during lamellipodium retrograde flow, a local retraction of actin branched network. In turn formation of newly focal complexes is followed by the advance of lamellipodium during cell ruffling. Experimental data suggest that those FA that originates from micron sized focal complex undergo maturation. FAs emerge as diverse protein networks that provide actin cytoskeleton structural integrity and the dynamic association with the ECM to facilitating cell migration and spreading through continuous regulation and the dynamic interaction with actin.
1.4 Cell Cytoskeleton
The interactions between integrin-mediated adhesions and the actin cytoskeleton are bidirectional:
cytoskeletal forces regulate the assembly and maturation of adhesions (see above), and at the same time, the growing adhesions can regulate the assembly of the actin system .
Actin assemblies into a wide variety of structures (fig. 1.3) which are able to support cellular integrity. It can be subdivided into five categories:
(1) lamellipodial networks at the leading edge of the cell, (2) filopodial bundles,
(3) the cortical actin shell beneath the plasma membrane,
(4) the contractile actin ring located at the divisionplane during cytokinesis (5) contractile filamentous actin.
Last category was commonly denoted as “stress fibres”, structures associated at their termini with FAs and maintain an isometric tension, which is applied to the ECM through cellular adhesions . Stress fibers are the major contractile structures in many cultured animal cells like fibroblasts, smooth muscle, endothelial and some cancer cell lines.
Figure 1.3: Schematic representation of the different actin cytoskeleton assemblies within cells
Actin filaments are polar helical structures, with a rapidly growing barbed end and a slowly growing pointed end . Stress fibers are composed of bundles of 10–30 actin filaments, which are crosslinked together by a-actinin, typically in a bi-polar arrangement. As described before, these contractile structures are often anchored to focal adhesions.
Stress fibers can be divided into at least four different categories: dorsal and ventral stress fibers, transverse arcs and the perinuclear actin cap [30-31-32] (fig 1.4).
Dorsal stress fibers are anchored to focal adhesions at their distal ends. Unlike the other types of stress fibers, dorsal fibers are not contractile structure in fact as described in several work [32-34]
dorsal SFs were defined as a platform for the assembly of other stress fibers.
Transverse arcs are contractile curved actin filament bundles, not associated with focal adhesions.
They display a periodic a-actinin–myosin pattern which is typical for contractile actomyosin bundles. Retrograde flow rapresent a distinctive feature of these structures. This process consists in the continuous contraction of arcs from the leading edge towards the cell center [31-34].
Ventral stress fibers are mainly located at posterior part of the cell. They are contractile actomyosin bundle characterized by two focal adhesions at both end of stress fiber .
Recent studies elucidated the role of perinuclear actin cap in regulating nucleus shape in interphase cell, acting as mechanostrasducers to transform force from cell environment to the nucleus .
This cap is composed of contractile actin filament bundle which form a highly organized, dynamic and oriented structure .
Figure 1.4 Schematic representation of stress fiber network of motile mesenchymal cells
In their surrounding environment, cells are exposed to various external forces such as stretching (muscle cells), compression (bones) or shear flows (blood cells). In the past years it has become clear that these extracellular stimuli affect cell behavior by triggering specific intracellular molecular pathways. Unfortunately, most of these intracellular events are still poorly understood.
Many experimental observations revealed the existence of a regulatory mechanisms for the interplay between intracellular- generated forces and the mechanical properties of the extracellular environment. Cells’ ability to react to substrate mechanical properties is referred as mechanosensing. The first experimental evidence of mechanosensing dates back more than 30 years when Harris et al.  reported and measured myoblasts contractile forces on flexible rubber membranes. Following this first report, other authors focused on developing systems to analyze the dynamics of cell-generated forces. Many cellular structure as integrin/FA sites, G-protein, ion channels, cytoskeleton constituents and membrane biomolecules have all been identified as potential mechanosensors . These specialized biomolecules change their chemical activity state when they are mechanically distorted, converting mechanical energy into biochemical energy .
Single molecule force spectroscopy studies showed that individual peptide domains within protein found in the cytoskeleton underwent stepwise elongation when they were mechanically extended .
Physical forces can modulate the kinetics of protein-protein binding in living cells. For example integrin, as described above, are transmembrane receptors structurally connected to cytoskeleton thanks to which, cells pull on their surrounding and probe the stiffness of extracellular environment.
As a consequence of the applied force, integrin signaling induces a reorganization of cytoskeleton architecture.
Moreover FAs dynamics via actomyosin contraction transmit force to substrate. So the material- cytoskeleton crosstalk involves force exchange between cells and substrate . Therefore, understanding the mechanism of cell’s interaction with natural or artificial surfaces should be a fundamental requirement when designing biomaterial to stimulate specific intracellular pathways.
The mechanical properties of the material represent a relevant aspect of the dynamic reciprocity between adhesion plaques growth and substrate deformation. It has been reported that cells have a have a higher proliferation rates on stiffer material then softer. Moreover cells migrate faster on soft substrates while they are more stationary on stiff substrate. According to this view, patterning of mechanical properties may be used to control cell behaviour.
1.6 Substrate Topography
A consistent number of studies reported that cell behavior is strongly influenced by material topographic texture. In vivo contexts, extracellular environment represents a set of topografic signals, perceived by cell at different length scale. Fibrils and fiber bundles (collagen and fibrin), rough surfaces (crystal deposit in bone) and porous membranes (basement membranes) represent examples of natural topographies. So topographical signals are not to be considered in vitro artifacts but they play a relevant role in cell-material interaction through direct alteration in several cellular processes.
Recent advancements in micro and nanofabrication technologies made it possible to imprint on top of substrate surface topographic feature favoring the study of the role of topography in cell–material interaction. Soft lithography [40-41], electron beam lithography  and nano-imprint lithography  can imprint topographic patterns with huge spatial resolution (of a few nanometers).
To describe material topography-cell interactions, it is appropriate to differentiate between length scales that might elicit different responses, consequently topographic features are generally subdivided into macro-micro- and nanoscale topography
Macrotopography refers to topographies features exhibiting characteristic dimensions that surpass those of cells (tens of micrometers) providing a geometric confinement of them. Usually microtopography is related to the use of surface roughness whose feature varing from few micron to 100 micron. Fabrication process as welding or laser cutting modify devices surface in order to regulate cell attachment.
Concerning nanotopography Lamers et al. [44-45] demonstrated that 70 nm represents a limit scale dimension under which topographic signal begin to be ineffective. So within the dimensional range of 70 nm and 2-5 µm topographic features approximate those of cell’s sensorial organelles such as FAs and filopodia, affecting cellular processes regulated by these structures.
Many authors reported that topographic substrate modification induced a nonuniform deposition of serum proteins on anisotropic patterned surface. Usually, fibronectin, vitronectin or collagen are adsorbed on the top surface of material. Braber et al.  and Recum et al.  thought that different surface energies on anisotropic patterned surface regions induce selective adsorbed of ECM proteins on the top of substrate topography. When contacting such surfaces, cells may recognize the anisotropic protein distribution on the top surfaces of the patterns. More and more researches have proved that the topography of the surface can influence significantly not only the distribution and adsorption but also the conformation and the activity of proteins [48, 49]. However, the processes that mediate cellular reaction to nanoscale surface structures are not well understood.
The use of micro/nanometric groove patterns is a method to mimic in vitro the topographical cues exposed to cell in extracellular environment in in vivo contexts. Cells seeded on grooved substrates usually acquire an elongated morphology and alignment to groove direction, reproducing in vivo tissue organization, facilitating active self assembly of ECM molecules enhancing cell attachment and polarization rate. A wide range of cell types such as fibroblasts , osteoblast , nerve cells  and MSCs  respond dramatically to grooved substrates.
Topography surface features are defined by three characteristic dimensions, namely ridge (or groove) width, inter-feature length (or pitch) and depth.
Furthermore, topographic patterns create surfaces that are readily accessible for cell lamellipodia and filopodia, such as the top of ridges or pillars, as well as impervious recesses, such as the bottom of grooves and pits. The accessibility of a given region to the cell membrane and its protrusions depends on the geometric characteristic of the pattern, i.e. the feature depth and pitch. Braber et al.
, Meyle et al. and Matsuzaka et al. reported that on microgroove patterns, focal adhesions formation occur predominantly on the top of the ridge due to the restriction imposed by steric hindrance. Furthermore orientation of FA plaques is affected by the presence of micro- nanograted substrate . The use of nanogroove substrates induces FAs maturation along the ridges  or at the groove/ridge boundaries  In this context many works investigate the effect of ridge/groove dimensions that are able to induce a cell alignment by FAs polarization. Teixeira et al.  observed that rearranging the FA distribution, epithelial cells switch from parallel to perpendicular alignment on grooved substrate when features decreased in pitch size from 4000 to 400 nm.
The molecular mechanism governing cell alignment is not fully characterized. In particular the crosstalk between topographic signals and cytoskeleton is not systematically described.
1.7 Aims and outcomes
The aim of this Thesis is to gain a deeper insight into the material-cytoskeleton crosstalk in order to design novel biomaterials which effectively control cell behavior in terms of cell polarization, migration and matrix deposition.
As discussed above several studies described the effects of mechanical and topographical feature on specific cellular processes. In particular cell adhesion and migration are affected by substrate surface feature. In these studies the effect of nanotoprografic feature have been well characterized but the intrinsic mechanism that induce cell to response to substrate features were still unknown.
This Thesis highlights the importance to improve the knowledge on cell material crosstalk with the aim of developing third generation devices (CIMs). In particular:
We present an innovative and simple soft UV lithographic method ‘‘Fill-Molding In Capillaries’’(FIMIC) that combines soft lithography with capillary force driven filling of micro-channels to create smooth hydrogel substrates with a 2D micro-pattern on the surface.
Within this study, smooth hydrogel surfaces displaying locally varied elasticity regions have been successfully achieved and applied in cell culture for cell guidance and durotaxis studies.
We study the effect of nanograted substrates on FA dynamics-cytoskeleton assembly- nuclear shape by time lapse live imaging in order to better understand the intrinsic mechanisms that regulate cell and nuclear polarization.
We investigated the synergistic effect of topographic signals and chemical characteristics on cell adhesion and migration. To this aim, we used micrograted polydimethylsiloxane (PDMS) substrates having feature dimension that might in principle interfere with the cell probing machinery, whereas surface chemical modifications were performed to modulate hydrophobic / hydrophilic properties by means of oxygen plasma treatment in order to affect focal adhesion formation and maturation.
We observed an intimate correlation between cell alignment and extracellular matrix production. In particular we studied the effect of cell migration on collagenous matrix production. To this aim we used nanograted substrate in ordered to produce a cell multilayer whose collagen fibers have a predefined spatial distribution.
 Esposito M, Worthington HV, Coulthard P. Interventions for replacing missing teeth: dental implants in zygomatic bone for the rehabilitation of the severely deficient edentulous maxilla.
Cochrane Database Syst Rev.2005;CD004151.
 Brooks KR, Capo JT, Warburton M, Tan V. Internal fixation of distal radius fractures with novel intramedullary implants. Clin Orthop Relat Res. 2006;445:42–50.
 Langer R, Vacanti JP. Tissue Engineering. Science 1993;260:920‐926
 Bonassar LJ, Vacanti CA. Tissue engineering: the first decade and beyond. J Cell Biochem Suppl. 1998;30-31:297-303
 Saxena AK, Marler J, Benvenuto M, Willital GH, Vacanti JP. Skeletal muscle tissue engineering using isolated myoblasts on synthetic biodegradable polymers: preliminary studies.
Tissue Eng. 1999 Dec;5(6):525-32.
 Lanza RP, Langer RS, Vacanti J. Principles of tissue engineering. 2nd ed. San Diego, CA ::Academic Press, 2000.
 Saltzman WM. Tissue Engineering: principles for the design of replacement organs and tissues.
1st ed. Oxford: Oxford University Press, 2004.
 Blitterswijk CAv, Thomsen P. Tissue engineering. 1st ed. Amsterdam; Boston:
Elsevier/Academic Press, 2008
 Fong P, Shin'oka T, Lopez‐Soler RI, Breuer C. The use of polymer based scaffolds in tissue engineered heart valves. Progress in Pediatric Cardiology 2006;21(2):193‐199
 Nesic D, Whiteside R, Brittberg M, Wendt D, Martin I, Mainil‐Varlet P. Cartilage tissue engineering for degenerative joint disease. Advanced Drug Delivery Reviews 2006;58(2):300‐322  Matsumura G, Hibino N, Ikada Y, Kurosawa H, Shin'oka T. Successful application of tissue engineered vascular autografts: clinical experience. Biomaterials 2003;24(13):2303‐2308
 Macchiarini P, Jungebluth P, Go T, Asnaghi MA, Rees LE, Cogan TA, et al. Clinical transplantation of a tissue‐engineered airway. The Lancet 2008;372(9655):2023‐2030
 Suska, F., Emanuelsson, L., Johansson, A., Tengvall, P. & Thomsen, P. (2007). Fibrous capsule formation around titanium and copper. J Biomed Mater Res A 85, 888-96
 Andersson, M., Suska, F., Johansson, A., Berglin, M., Emanuelsson, L., Elwing, H. &
Thomsen, P. (2007). Effect of molecular mobility of polymeric implants on soft tissue reactions: An in vivo study in rats. J Biomed Mater Res A 84A, 652-660
 Baxter, L. C., Frauchiger, V., Textor, M., ap Gwynn, I. & Richards, R. G. (2002). Fibroblast and osteoblast adhesion and morphology on calcium phosphate surfaces. Eur Cell Mater 4, 1-17
 Ventre M, Causa F, Netti PA. Determinants of cell-material crosstalk at the interface: towards engineering of cell instructive materialsJ R Soc Interface. 2012 Sep 7;9(74):2017-32.
 Schwarz, U. S., Erdmann, T. & Bischofs, I. B. (2006). Focal adhesions as mechanosensors: the two-spring model. Biosystems 83, 225-32
 Triplett, J. W. & Pavalko, F. M. (2006). Disruption of alpha-actinin-integrin interactions at focal adhesions renders osteoblasts susceptible to apoptosis. Am J Physiol Cell Physiol 291, C909- 21
 Dettin, M., Conconi, M. T., Gambaretto, R., Bagno, A., Di Bello, C., Menti, A. M., Grandi, C.
& Parnigotto, P. P. (2005). Effect of synthetic peptides on osteoblast adhesion. Biomaterials 26, 4507-15
 Pieta K. Mattila and Pekka Lappalainen. (2008). Filopodia: molecular architecture and cellular functions. Nat Rev Mol Cell Biol. 2008 Jun;9(6):446-54.
 Lim, J. Y., Dreiss, A. D., Zhou, Z., Hansen, J. C., Siedlecki, C. A., Hengstebeck, R. W., Cheng, J., Winograd, N. & Donahue, H. J. (2007). The regulation of integrinmediated osteoblast focal adhesion and focal adhesion kinase expression by nanoscale topography. Biomaterials 28, 1787-97  Bershadsky, A. D., Ballestrem, C., Carramusa, L., Zilberman, Y., Gilquin, B., Khochbin, S., Alexandrova, A. Y., Verkhovsky, A. B., Shemesh, T. & Kozlov, M. M. (2006b). Assembly and mechanosensory function of focal adhesions: experiments and models. Eur J Cell Biol 85, 165-73  Cavalcanti-Adam, E. A., Volberg, T., Micoulet, A., Kessler, H., Geiger, B. & Spatz, J. P.
(2007). Cell spreading and focal adhesion dynamics are regulated by spacing of integrin ligands.
Biophys J 92, 2964-74.
 Cohen, D. M., Chen, H., Johnson, R. P., Choudhury, B. & Craig, S. W. (2005). Two distinct head-tail interfaces cooperate to suppress activation of vinculin by talin. J Biol Chem 280, 17109-17  Garcia, A. J. (2005). Get a grip: integrins in cell-biomaterial interactions. Biomaterials 26, 7525-9
 Michele A. Wozniak, Katarzyna Modzelewska, Lina Kwong, Patricia J. Keely (2004). Focal adhesion regulation of cell behavior. Biochimica et Biophysica Acta 1692, 103– 119
 Geiger B, Spatz JP, Bershadsky AD. Environmental sensing through focal adhesions. Nat Rev Mol Cell Biol. 2009 Jan;10(1):21-33
 Zimerman, B., Volberg, T. & Geiger, B. (2004). Early molecular events in the assembly of the focal adhesion-stress fiber complex during fibroblast spreading. Cell Motil Cytoskeleton 58, 143-59  Pollard, T. D. and Cooper, J. A. (2009). Actin, a central player in cell shape and movement.
Science 326, 1208-1212
 Cramer, L. P., Siebert, M. and Mitchison, T. J. (1997). Identification of novel graded polarity actin filament bundles in locomoting heart fibroblasts: implications for the generation of motile force. J. Cell Biol. 136, 1287-1305
 Small, J. V., Rottner, K., Kaverina, I. and Anderson, K. I. (1998). Assembling anactin cytoskeleton for cell attachment and movement. Biochim. Biophys. Acta. 1404, 271-281
 Khatau, S. B., Hale, C. M., Stewart-Hutchinson, P. J., Patel, M. S., Stewart, C. L., Searson, P.
C., Hodzic, D. and Wirtz, D. (2009). A perinuclear actin cap regulates nuclear shape. Proc. Natl.
Acad. Sci. USA 106, 19017-19022
 Tojkander, S., Gateva, G., Schevzov, G., Hotulainen, P., Naumanen, P., Martin, C., Gunning, P.
W. and Lappalainen, P. (2011): A molecular pathway for myosin II recruitment to stress fibers. Curr.
Biol. 21, 539-550
 Hotulainen, P. and Lappalainen, P. (2006). Stress fibers are generated by two distinct actin assembly mechanisms in motile cells. J. Cell Biol. 173, 383-394.
 Harris, A. K., Wild, P. & Stopak, D. 1980 Silicone rubber substrata: a new wrinkle in the study of cell locomotion. Science 208, 177–179.
 Mack, P. J., Kaazempur-Mofrad, M. R., Karcher, H., Lee, R. T. & Kamm, R. D. (2004).
Force-induced focal adhesion translocation: effects of force amplitude and frequency. Am J Physiol Cell Physiol 287, C954-62
 Ingber DE Cellular mechanotransduction: putting all the pieces together again. FASEB J. 2006 May;20(7):811-27
 Li, H., Linke, W. A., Oberhauser, A. F., Carrion-Vazquez, M.,Kerkvliet, J. G., Lu, H., Marszalek, P. E., and Fernandez, J. M.(2002) Reverse engineering of the giant muscle protein titin.Nature418,998 –1002
 Nicolas A. Physically based principles of cell adhesion mechanosensitivity in tissues. Rep Prog Phys. 2012 Nov;75(11):116601.
 den Braber, E. T., de Ruijter, J. E., Ginsel, L. A., von Recum, A. F. & Jansen, J. A. 1998 Orientation of ECM protein deposition, fibroblast cytoskeleton, and attachment complex components on silicone microgrooved surfaces. J. Biomed. Mater. Res. 40, 291–300.
 Yim, E. K., Reano, R. M., Pang, S. W., Yee, A. F., Chen, C. S. & Leong, K. W. 2005 Nanopattern-induced changes in morphology and motility of smooth muscle cells.Biomaterials 26, 5405–5413.
 Dalby, M. J., Biggs, M. J., Gadegaard, N., Kalna, G., Wilkinson, C. D. & Curtis, A. S. 2007 Nanotopographical stimulation of mechanotransduction and changes in interphase centromere positioning. J. Cell. Bichem. 100, 326–338.
 Gaubert, H. E. & Frey,W. 2007 Highly parallel fabrication of nanopatterned surfaces with nanoscale orthogonal biofunctionalization imprint lithography. Nanotechnology 18, 135 101–135 107.
 Lamers, E., van Horssen, R., te Riet, J., van Delft, F. C., Luttge, R., Walboomers, X. F. &
Jansen, J. A. 2010 The influence of nanoscale topographical cues on initial osteoblast morphology and migration. Eur. Cell Mater. 20, 329–343
 Loesberg, W. A., te Riet, J., van Delft, F. C., Scho¨n, P., Figdor, C. G., Speller, S., van Loon, J.
J., Walboomers,X. F. & Jansen, J. A. 2007 The threshold at which substrate nanogroove dimensions may influence fibroblast alignment and adhesion. Biomaterials 28, 3944–3951.
 den Braber E T, Ginsel L A, von Recum A F, et al. Orientation of ECM protein deposition, fibroblast cytoskeleton, and attachment complex components on silicone microgrooved surfaces. J Biomed Mater Res, 1998, 40: 291―300
 Recum A F, van Kooten T G. The influence of micro-topography on cellular response and the implications for silicone implants. J Biomater Sci Polym Ed 7, 1995, 7: 181―198
 Song W, Chen H. Protein adsorption on materials surfaces with nano-topography. Chinese Sci Bull, 2007, 52: 3169―3173
 Roach P, Farrar D, Perry C C. Surface tailoring for controlled protein adsorption: effect of topography at the nanometer scale and chemistry. J Am Chem Soc, 2006, 128: 3939―3945
 Dalby, M. J., Riehle, M. O., Yarwood, S. J., Wilkinson, C. D. & Curtis, A. S. (2003c). Nucleus alignment and cell signaling in fibroblasts: response to a micro-grooved
topography. Exp Cell Res 284, 274-82
 Lenhert, S., Meier, M. B., Meyer, U., Chi, L. & Wiesmann, H. P. (2005). Osteoblast alignment, elongation and migration on grooved polystyrene surfaces patterned by
Langmuir-Blodgett lithography. Biomaterials 26, 563-70
 Yim, E. K., Pang, S. W. & Leong, K. W. (2007). Synthetic nanostructures inducing differentiation of human mesenchymal stem cells into neuronal lineage. Exp Cell Res 313, 1820-9  Dalby, M. J., McCloy, D., Robertson, M., Agheli, H., Sutherland, D., Affrossman, S. & Oreffo, R. O. (2006b). Osteoprogenitor response to semi-ordered and random nanotopographies.
Biomaterials 27, 2980-7.
 Meyle J, Gultig K, Brich M, et al. Contact guidance of fibroblasts on biomaterial surfaces. J Mater Sci Mater Med, 1994, 5: 463―466
 Matsuzaka K, Walboomers F, de Ruijter A, et al. Effect of microgrooved poly-l-lactic (PLA) surfaces on proliferation, cytoskeletal organization, and mineralized matrix formation of rat bone marrow cells. Clin Oral Implant Res, 2000, 11: 325―333
 Teixeira, A. I., Nealey, P. F. & Murphy, C. J. (2004). Responses of human keratocytes to micro- and nanostructured substrates. J Biomed Mater Res A 71, 369-76.
 Teixeira, A. I., Abrams, G. A., Bertics, P. J., Murphy, C. J. & Nealey, P. F. (2003). Epithelial contact guidance on well-defined micro- and nanostructured substrates. J Cell Sci 116, 1881-92  Wojciak-Stothard, B., Curtis, A., Monaghan, W., MacDonald, K. & Wilkinson, C. (1996).
Guidance and activation of murine macrophages by nanometric scale topography. Exp Cell Res 223, 426-35.
 Teixeira, A. I., McKie, G. A., Foley, J. D., Bertics, P. J., Nealey, P. F. & Murphy, C. J. (2006).
The effect of environmental factors on the response of human corneal epithelial cells to nanoscale substrate topography. Biomaterials 27, 3945-54.
Molding Micropatterns of Elasticity on Peg-Based Hydrogels to Control Cell Adhesion and Migration
This work arose from the collaboration with Prof. M. C. Lensen of the Technische Universität Berlin · Institut für Biotechnologie and it was published on Advanced Engineering Material in October 2011.
It is well known that surface characteristics such as biofunctionality, topography, and elasticity have a profound effect on cell adhesion, spreading, migration, and intracellular processes, which can also direct cell differentiation. [1–5]
Therefore, understanding of the mechanisms of cells’ interaction with natural or artificial surfaces is a fundamental requirement when designing biomaterials for different biomedical applications, e.g.
tissue engineering, drug delivery, or diagnostics. Several systems and techniques have been introduced which can be applied for a systematic in vitro study of the correlation between substrate characteristics and cell reactions. Yet, although it is the combination of several substrate properties that directs the cellular outcome, most of the in vitro studies so far have varied only one parameter at atime, e.g. employing either chemical or physical surface patterns.[1,6–8]
Lithographic techniques such as photolithography, which were developed at first for minimizing electronic devices, have emerged as powerful tool toward the engineering of biosurfaces.
However, and to defeat shortcomings of conventional techniques on soft materials, development has pushed fabrication techniques such as soft lithography which have rendered successful micro- and nano- structures of a wide variety of soft materials, including the one described here.[10–15]
Chemical patterning to create cell responsive patterns can be achieved by controlled incorporation of cell-specific responsive ligands.[5,16–18] Lately, many successful strategies
have been developed to create gradient elasticity on substrates destined to cell-based assays;
photolithographic patterning, [19–22] soft lithography,[23,24] and capillary in microchannels 
have been effectively utilized to gradient the elasticity of e.g., PDMS (polydimethylsiloxane) and PAAm (polyacrylamide) using mainly silicon and glass as base substrate.
Although there is significant evidence of the influence of mechanical and tensile properties of the substrate on the host response, e.g. cell adhesion and motility are highly dependent on the substrate’s rigidity,[7,26,27] the use of chemical modification of the surfaces with specific ligands
So far, elasticity variations have been fabricated mostly in a gradual fashion, for example by employing a photomask over a UV-curable polymer. Lo and coworkers, nevertheless, have described binary patterns of stiffness and consequent ‘‘durotaxis’’ experiments have demonstrated the migration of cells in the direction of stiffer regions of the substrate.
Such surfaces with a rigidity boundary are exceptionally interesting to elucidate cells’
mechanosensing of relatively sharp contrasts in stiffness. With our surface patterning method we are able to take this concept of contrast sensing a step further and investigate cell migration on substrates with multiple boundaries of stiffness variations. As a material of choice we have employed hydrogels, which can be tailored in their mechanical properties by virtue of variations in their crosslinking density.
Over the past years, much attention has been paid to hydrogel materials as potential synthetic biomaterials due to their biocompatibility promoted by the high water content and physicochemical similarities to native extra cellular matrix.[31–33] Hydrogels have found many applications, for instance, in tissue engineering scaffolds, implantable devices, and drug delivery. The ability to swell makes this kind of material eligible for use in drug delivery and immobilization of proteins, peptides, and other biological compounds.[34–39]
In the same way, the possibility of changing the inner architecture by varying crosslinking density of the network can dramatically impact polymer diffusivity and permeability, degradation rate, equilibrium water content (EWC), elasticity, and modulus.[31,40–43] encompassing the elastic moduli found in human tissue, i.e. ranging from a few kPa to a few GPa.[44,45]
As biomaterials, hydrogels provide bulk and mechanical support for cellular attachment since they can be designed as required of the construct in terms of mechanical and chemical properties.[42,46]
A wide variety of natural and synthetic chemical building blocks have been used to synthesize many different hydrogel materials with engineered surface chemistry, controlled porosity, and crosslinking density. Especially poly(ethylene glycol), PEG, based hydrogels are very popular for biomedical applications. They are highly hydrated, oxygen permeable and protein absorption resistant, and also often used as coating material to render surfaces bioinert.[47–49] Nevertheless, PEG’s renown, non-adsorptive properties can be modulated by different factors, e.g. by the addition of peptide sequences, chemical, or topographical cues, etc. In fact, we have recently discovered that the PEG-hydrogel surface loses its cell anti-adhesive properties when it is topographically patterned. The so-called contact guidance is an outstanding example of the important role of nano- and micro scale structures in cell adhesion and migration processes.[52–60] With the development of FIMIC (FIll-Molding In Capillaries), which is a novel technique that partly relies on the soft lithography technique MIMIC (MIcroMolding In Capillaries), we intend to provide a versatile strategy to obtain a defined, two-dimensional elasticity pattern on an otherwise smooth
substrate in a simple, low-cost, and reproducible manner. The PEG-based biocompatible hydrogel material herein was prepared via UV photopolymerization of starPEG acrylate macromonomers in the presence of a photoinitiator and eventually a crosslinker (CL). Tuning of the elasticity of the substrate was easily done by varying crosslinking density on the final hydrogel material.
The PEG-hydrogel here presented has been reported in our group to be non adsorptive, biocompatible, and without further chemical modification or bioactivation, able to induce different cellular responses. Furthermore, patterning on its surface has been proved down to a few nanometers. Within this study, smooth hydrogel surfaces displaying locally varied elasticity regions have been successfully achieved and applied in cell culture, i.e. for cell guidance and durotaxis studies.
Hydrogel Preparation and Characterization
The hydrogel material in this method was formed by UV photocrosslinking of multiacrylate starPEG macromonomers in the presence of benzoin methyl ether (BME) as photinitiator (PI) and pentaerythritol triacrylate (PETA) as a CL as described in ref.[13,51]. Briefly, acrylate functional groups were introduced in star-shaped sP(EO-stat-PO) (Mn 12 500 Da, Dow Chemicals, The Netherlands) macromonomers which, in the presence of a photoinitiator could take part in photoinitiated crosslinking reactions to yield polymer networks. In order to fabricate different stiffness, pre-curing mixtures were prepared by mixing Acrylate terminated starPEG macromonomer (Acr- sPEG) with varying amounts of PI (0.5–1 wt%) and CL (5–10 wt%) with respect to the amount of polymer in the presence of acetone as a solvent. Once the solvent was evaporated under nitrogen stream, the pre-curing mixture
could be stored in the dark at 4- 8°C for as long as 3 weeks without deterioration. UV curing was performed using 20 min of irradiation (λ=365 nm; W=1.20mW· cm–2). As a result of UV curing, a 3D transparent crosslinked hydrophilic network was obtained. Within this text the three different compositions employed will be denoted based on their elasticity as soft, medium, and stiff, respectively (see Table 1).
Mechanical analysis of the resultant hydrogels was performed on dry as well as on hydrated samples. The bulk gels were allowed to swell in seral (double-distilled) water for24 h prior use to
ensure EWC. Swelling ratio (SR) was determined by the weight ratio of the bulk gel before and after swelling.
Rheology experiments were performed on a Dynamic Stress Rheometer DSR (Rheometrics Inc., New Jersey, USA) using rotating parallel plates at room temperature. Storage and loss moduli were measured as a function of the frequency (from 0.05 to 10 Hz) in a constant strain mode. Young’s modulus (E) was then calculated from the elastic shear modulus (G) using the rubber elasticity theory E=3G’. Dynamic Mechanical Analyzer (DMA Q800 TA Instruments) in compression mode was employed to determine the
Young’s moduli from the slope in the linear region of the strain–stress curve. A stress ramp of 0.5N·min–1, with initial force 0.01N was applied up to 30% strain. The experiments in swollen state were performed in similar conditions using the submersion compression clamp.
Table 1: Notation assigned to the different hydrogel material based on the composition of the pre-curing mix
Micrometer Hydrogel Stamp Fabrication
Silicon masters were prepared from silicon wafers by conventional photolithographic techniques with trenches as relief (Amica, Aachen, Germany). For different masters, feature design consisted on diverse spacing (5, 10, 20 mm) and groove width (10, 20, 50 µm) at constant depth (10 µm) (see Table 2). Silicon wafers were rinsed with acetone, water, and isopropanol and dried under a mild stream of nitrogen before use. Within the text the notation of the silicon master will be e.g., 20_10 mm (spacing_groove width), resulting in hydrogel mold with e.g., 10_20 µm patterns.
The selected hydrogel pre-curing mixture was dispensed on the silicon master under inert atmosphere and exposed to UV light for 20 min. Following curing, the transparent polymeric film with inverse relief compared to that on the silicon master was peeled off mechanically. The replicas displayed a constant spacing of 10, 20, or 50 µm between grooves of variable width, i.e. 5, 10, or 20 µm, which were filled in the subsequent patterning step.
Table 2: Silicon master design and dimensions
2D Microelasticity Pattern Fabrication by the FIMIC Process
A small amount of the second hydrogel precursor of the composite was carefully dispensed at the edge of the open channels of the PEG stamp hydrogel placed upside down on a glass slide (see Fig.
3). The viscous liquid mixture was allowed to fill the capillaries, in the dark and inert atmosphere for 30 min after which the assembly was exposed to UV light for 20 min. After exposure time was complete the hybrid construct was easily detached from the glass substrate mechanically and turned upside down to proceed with surface characterization and cell culture. The resultant polymer composite was a robust, free standing, transparent film.
The surface of the hybrid hydrogel structure was investigated by several techniques, FESEM and AFM in dry state and eventually optical microscopy on the sample in water. Notation of the assembly will be done as follows, e.g. ‘‘soft (20 µm) in stiff (10 µm)’’, meaning that the surface contains 20 µm wide soft lines alternated with the 10 µm wide stiff lines of the stamp. The composition and patterning dimensions of all hybrid constructs prepared in this study are listed in Table 3. The samples were handled with Teflon tweezers and cut with razor blades with no further cares. Prior to use, glass slides used as substrates were cleaned by rinsing in acetone, water, and isopropanol and dried under a mild stream of nitrogen in order to eliminate organic residues.
Table 3: Notation of the hybrid hydrogel samples
Atomic Force Microscopy (AFM)
Images were taken in tapping mode using standard silicon cantilevers (k=40 N·m–1, f=300 kHz;
Nanoworld, Neuchatel, Switzerland) on a Digital Instrument Multimode equipped with a NanoScope IIIa controller (Veeco Instruments, SantaBarbara, CA) in air. Data were edited using NanoScope III v5.12r5 software (Veeco Instruments, Santa Barbara, CA). The images were flattened but not further modified.
Fibroblast Cell Culture
Mouse connective tissue fibroblast cell line NIH L929 was used for the experiments (DMSZ, Braunschweig, Germany). Cells were cultured in RPMI-1460 medium supplemented with 10% fetal bovine serum and 1% penicillin/streptomycin at 37°C in a 5% CO2 supplied incubator. The culture medium was changed every 2 days. Cells were harvested with 0.25% trypsin/EDTA. For the cultivation experiments the inoculation density was 50 000 cells ·cm2. (Samples were cultivated in well plates with a well area of 1 cm2 and 1ml of a 50 000 cells ·ml–1 suspension was added to the wells on top of the samples). Samples were rinsed with sterile water and bufferprior to cell seeding.
All reagents were purchased from PAA, Cölbe, Germany.
For immunological staining of the cytoskeleton, cells were fixed in 4.0% formaldehyde at pH 7 (Carl Roth, Karlsruhe, Germany), permeabilized with 0.1% Triton X-100 (Sigma–Aldrich Chemie, Munich, Germany) and blocked in 1% BSA in PBS (PBSA). To visualize cell morphology cells were labeled with tetramethylrhodamine isothiocyanate (TRITC)-conjugated phalloidin (1:500) for 30–45 min followed by DNA staining with 4’6-diamidino-2-phenylindole (DAPI) (1:1000) for 5 min (Chemicon).
Optical and Fluorescent Microscopy
Light microscopy images were taken with an inverted Axiovert 100A Imaging microscope (Carl Zeiss, Goettingen, Germany). Cell adhesion and spreading were monitored by means of fluorescent microscopy with an Axio Observer Z1, equipped with an Apo Tome system to achieve optical sectioning through the fluorescent sample. Pictures were taken using an AxioCam MRm digital camera and analyzed using the AxioVisionV4.6/V4.7 software package (Carl Zeiss, Goettingen, Germany).
Field Emission Scanning Electron Microscopy (FESEM)
Images were taken by a high resolution field emission scanning electron microscope (FESEM; S- 4800, Hitachi, Krefeld, Germany). In the case of hydrogel substrates an accelerating voltage of 1.5 kV and varying working distance (6.5 to 10mm) were used. In the case of cell imaging 1.0 kV and a working distance of 8mm were the microscope parameters. Cell containing samples were prepared as follows: after a cultivation time of 24 h, the substrates with the L929 cells were rinsed three times with PBS and fixed with 4.0% formaldehyde for at least 30 min and dehydrated by incubating consecutively in 50, 70, 90, and 100% ethanol.
Cell Migration Experiments
Videos of migrating cells were obtained by acquiring images (approximately 700µm_600 µm) on selected regions of the L929 populated hydrogel gel [stiff (10µm) in soft (20µm)] every 10 min
a mini-incubator mounted on an automated stage (PRIOR, Rockland, MA) and a CoolSnap Camera (Photometrics, Tucson, AZ). Cell tracks were reconstructed from the time lapse videos using Metamorph software (Molecular Device, Sunnyvale, CA).
2.3 Results and Discussion
To fabricate our hydrogel system we use a previously described procedure (see Experimental Part).
The macromonomer of choice is a six armed Acr-sP(EO-stat-PO) (Mn 12 500 Da) which can undergo radical crosslinking initiated by UV light in the presence of a photoinitiator. Varying the amount of initiator and eventually adding a CL molecule to the pre-curing mixture results in an increase of the network density, the resulting polymer is an insoluble highly crosslinked network able to take up large amounts of water (or biological fluids), hence a hydrogel by definition.
So far, hydrogels have been described ranging in elasticity from few Pa to hundreds of kPa. As several hydrogels can be fabricated with different elasticities yet the same chemistry, they represent a useful substrate to study elasticity-dependent cell behavior (mechanotransduction).
In the present study we prepare smooth hydrogel substrates which exhibit two different, tuneable elasticities on their surface, arranged in a specific pattern. Three hydrogel compositions were prepared for this purpose in order to obtain a relevant elasticity range, although mainly the combinations of softest and the stiffest gel were applied in the experiments. The fabrication of different elasticity hydrogels was done by varying the amount of PI and CL in the liquid pre-curing mixtures as specified in Table 1. In order to assess the impact of PI and CL concentration on the resulting hydrogel, the elasticity range of the bulk gels was investigated by rheology applying the rubber elasticity theory and by dynamic mechanical analysis for comparison.
The swelling behavior of the materials was investigated as well and represented by the SR in Figure 1; mechanical properties in hydrated conditions were determined after 72 h in water. A graphical representation of the mechanical analysis can be seen in Figure 1, where Young’s Moduli (E) is plotted against the composition of the pre-curing mixture.
From the measurements in the dry state, DMA data provided 0.24±0.02MPa and 2.50±0.50MPa for the soft and stiff hydrogel, respectively, and these results compare well to those from rheological determinations. Young’s moduli increase with increasing the crosslinking density of the network, which implies formation of a denser network.
Normally, an increase in crosslinking density is associated with a decrease in the water uptake. As expected, the SR values clearly decrease with increasing crosslinking density of the gel network [Fig. 1(b)]. Further, the swelling makes the gels softer; the stiffness of the swollen hydrogel decreases to typically half of the dry hydrogel value. All samples were transparent polymers before and after swelling in water, still easy to handle as free-standing films. Those results prove the ability of this hydrogel to vary in rigidity over a quite large range, without compromising the transparency of the polymer as required for further applications, e.g. live imaging of cell culture on the samples by optical microscopy and immunological staining experiments by fluorescence microscopy using inverted microscopes.
Figure 1: a) Elastic modulus as a function of gel composition as obtained from DMA (solid symbols) and rheology (open symbols); circles and diamonds represent the values for hydrated and dry hydrogels,
respectively. b) SR represented as a function of the composition
For the preparation of the PEG-hydrogel mold, the Acr-sP(EO-stat-PO) mix of choice was cured under UV light for 20 min against mm-sized groove structured silicon master (e.g. 20_10 mm). As a result of the imprinting process, the micrometer design was transferred inversely into the surface of the cured polymer [Fig. 2, top].
Figure 2: Top: schematic representation of the micromolding process to fabricate a hydrogel replica. The electron micrograph on the right depicts a cross-section through the material, which is a negative copy of the
micropatterned silicon master (scale bar 25 mm). Electron micrographs a), b), and c) depict replicas from a 5_10 mm silicon master (thus bearing 5mm wide grooves, spaced by 10mm) using soft, medium, and stiff
hydrogel, respectively. Scale bars represent 50mm.
The free-standing polymeric micropatterned mold was placed upside down on a microscopy glass using tweezers and applied subsequently as the mold for the capillary filling process. Figure 3 shows a sketch of the experimental procedure of the new FIMIC method. In the second step, the capillary filling of the open channels of the PEG-hydrogel stamp were filled within 30min under inert atmosphere and cured into a solid elastomer. The hybrid film was lifted mechanically without residual polymeric material remaining on the glass slide. Delaminating of the composite was not observed, confirming that the integrity of the hybrids was not disrupted by shear or pulling forces that can be significant during release.
Figure 3: Schematic representation of the FIMIC method to prepare hybrid hydrogels with micropatterns of elasticity on the otherwise smooth surface
The versatility of this strategy and the material properties permitted the capillary filling process to be completed within 30 min for all dimensions tested. In all cases the resulting microfabricated substrate was a transparent freestanding polymeric film that could be easily manipulated with tweezers without further precautions. A smooth, micropatterned surface was expected provided by the set up. In Figure 4(a), the FESEM image of a hybrid structure ‘‘soft (20 µm) in stiff (10 µm)’’ is shown. The stripes corresponding to soft and stiff hydrogel can be recognized in the electron micrograph by their light and dark gray color, respectively. The image clearly demonstrates a binary pattern consisting of well-defined, parallel lines. An optical micrograph of the surface area is shown in Figure 4(c). The smoothness of the surface contour was verified by analyzing the cross-section profile on the AFM images (Inset in Fig. 4); on a span of 10 µm a negligible unevenness of <0.03 µm can be perceived.
Figure 4: Micrographs of hybrid hydrogel ‘‘soft (2mm) in stiff (10mm)’’ measured in dry state. Scale bars represent 50 mm. Recognized in light and dark gray are soft and stiff material, respectively. a) and b) FESEM images of the micro-patterned surfaces. In b) defects at the cutting edge of the hybrid sample are
shown; lines (of the soft material;light gray) that come loose from the mold (stiffer gel; dark gray) or are completely missing are clearly recognized. c) Optical micrograph. Inset: AFM cross-section profile of the
In order to verify that the binary pattern on the image indeed corresponds to alternating hydrogel material certain considerations must be taken into account. On the one hand, the mold should provide good ‘‘sealing’’ to the glass slide at the protruding areas to avoid creeping of the liquid underneath the mold during the capillary filling process, which would lead to the formation of a scum layer. On the other hand, diffusion of the second hydrogel precursor into the already crosslinked mold is not desired since blending of the two components could lead to a change in gel properties at the interfaces. To acknowledge those matters, we cut the substrate with a razor blade and examined the surface profile at the cutting edge. As can be observed in Figure 4(b) no trace of
lines are flexible, since 20 µm wide laminas can be separated and stand alone, apart from the stiff hydrogel frame, when they are mechanically disturbed, e.g. at the cutting edge. Nevertheless, delamination of the lines was rarely observed away from the edge. Thus it seems that the soft lines embedded in the stiff hydrogel stamp are neither chemically nor physically interconnected, however physically entrapped in the micrometer cavities, which is apparently quite adequate to keep them in place.
Since the substrates are destined to biological applications it is important to know how they respond in liquid media. We are aware that additional forces caused by e.g., the differential swelling of both materials might affect the reliability of the hybrid structure under water. Hydrogels in water are known to swell to larger size than initially in dry state showing decreasing values with stiffness (see Fig. 1 for SR depending on composition). Accordingly, one could expect that expansion forces encountered due to swelling may provoke the trapped lines to be pushed out of their initial location.
To that purpose, the resultant hybrid-hydrogel substrates were hydrated for as long as 3 days in distilled water and monitored afterwards.
FESEM images of the swollen samples were taken after gently wiping off the excess water of the hydrated samples. Figure 5(a) shows the image of the largely defect-free surface in comparison to an area with a defect in Figure 5(b). A clear binary pattern can be distinguished on the hydrogel surface.
However to a more faithful analysis, optical microscopy was the method of choice in order to characterize the integrity of the structures directly in water. It can be seen how the soft hydrogel stripes, recognized by the brighter lines are stable in the frame; still, delamination was observed to occur occasionally as well. [Fig. 5(d)]. No major deformation of the assembly seemed to be initiated by swelling expansion forces at the surface. Further inspection of the surfaces by means of AFM under water is in progress in order to visualize the possible effect of differential swelling on pattern dimensions and surface smoothness.
Figure 5: Hybrid hydrogel with pattern ‘‘soft (20mm) in stiff (10mm)’’ in hydrated state; a) and b) depict FESEM images; showing one line coming loose in image b). Light and dark gray are soft and stiff hydrogel,
respectively. c) and d) depict optical micrographs, revealing a defect area on the patterned surface in d).
Scale bars represent 50mm.
The described substrates have been applied for preliminary cell culture experiments with a murine fibroblast cell line (NIH L929). We wanted to assess whether the cells react in their adhesion and spreading behavior according to the pattern of elasticity, whereas they have been observed not to adhere at all on non-biofunctionalized, smooth hydrogel surfaces with uniform stiffness.
Fibroblasts were cultured on the hybrid surface for 24 h and monitored by optical microscopy, electron microscopy, and fluorescent microscopy after immunological staining.
Cells were seeded on various hybrid substrates with different line patterns created by either filling
‘‘stiff in soft’’ (Fig. 6, top) or ‘‘soft in stiff ’’ (Fig. 6, bottom). Also ‘‘stiff in stiff’’ samples were prepared as control samples (images not shown).
From the microscopy images one can clearly distinguish how cells seeded on smooth hybrid
6 show the clear alignment of single cells along the 10 µm stiffer lines, evident from Figure 6(b) where some stripes appear to be missing. The live optical micrograph in Figure 6(d) confirms selective cell adhesion and agglomeration on 50 µm stiffer regions, leaving the soft lines in between practically untouched. In order to visualize the cell morphology more precisely, the cell nucleus and the actin cytoskeleton were stained with DAPI (blue) and phalloidin (red), respectively. The fluorescence micrographs shown in Figure 6(c), (e), and (f) confirm the selective attachment on the stiffer regions. This cellular behavior was observed independent of the feature size; stiffer lanes as narrow as 5 µm (which is smaller than the cell’s own size) were effective (images not shown) and stripes as broad as 50 µm were recognized. This also implies that the elasticity sensing mechanism is not restricted to a border effect; it stretches over several micrometers.
Figure. 6. Fibroblast L2929 adhesion to hybrid hydrogel; cells selectively adhere to the stiffer areas of the samples. Top: ‘‘stiff in soft’’ samples, for example 10 µm stiff lines in soft moldwith 20 µm spacing as shown in the FESEM images in a) and b). Bottom: ‘‘soft in stiff’’ samples, for example 10 µm soft lines in stiff mold with 50 µm spacing as shown in d) and e). c), e), and f) show fluorescence micrograph; the cells were stained with DAPI and phalloidin, which appear as dark and light grey, respectively, to highlight the nucleus and the actin filaments of the cytoskeleton, respectively.
Notwithstanding the remarkable effectiveness of directing cell adhesion by the micropatterns of elasticity, we are also very interested in the dynamic mechanosensing processes leading to the eventual accumulation of the cells on the stiffer areas of the surface.
That’s why we have also performed cell migration experiments. From the tracking of several individual cells the preference for the stiffer lanes has been confirmed. In Figure 7(a), a few of such